#------------------------------------------------------------------------------
#$Date: 2016-02-13 20:28:24 +0100 (Sat 13 de Feb de 2016) $
#$Revision: 176429 $
#$URL: svn://www.crystallography.net/cod/cif/1/53/57/1535744.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1535744
loop_
_publ_author_name
'Iijima, K.'
'Marumo, F.'
'Takei, H.'
_publ_section_title
;
 Structural Changes of a Piezoelectric Crystal BaZnGeO~4~ on Thermal
 Phase Transition
;
_journal_issue                   1050
_journal_name_full               'Journal of the Ceramic Association, Japan'
_journal_page_first              67
_journal_page_last               72
_journal_paper_doi               10.2109/jcersj1950.91.1050_67
_journal_volume                  91
_journal_year                    1983
_chemical_formula_sum            'Ba Ge O4 Zn'
_chemical_name_systematic        'Ba Zn (Ge O4)'
_space_group_IT_number           182
_symmetry_space_group_name_Hall  'P 6c 2c'
_symmetry_space_group_name_H-M   'P 63 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.407
_cell_length_b                   5.407
_cell_length_c                   8.975
_cell_volume                     227.236
_citation_journal_id_ASTM        YGKSA4
_cod_data_source_file            Iijima_YGKSA4_1983_790.cif
_cod_data_source_block           Ba1Ge1O4Zn1
_cod_original_cell_volume        227.2364
_cod_original_formula_sum        'Ba1 Ge1 O4 Zn1'
_cod_database_code               1535744
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
x-y,x,z+1/2
-y,x-y,z
-x,-y,z+1/2
-x+y,-x,z
y,-x+y,z+1/2
-y,-x,-z+1/2
x-y,-y,-z
x,x-y,-z+1/2
y,x,-z
-x+y,y,-z+1/2
-x,-x+y,-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Ge1 Ge+4 0.6667 0.3333 0.4484 0.5 0.0
O2 O-2 0.6667 0.3333 0.25 1 0.0
O1 O-2 0.348 0 0.5 1 0.0
Zn1 Zn+2 0.6667 0.3333 0.4484 0.5 0.0
Ba1 Ba+2 0 0 0.25 1 0.0
